1 International Journal of Pharmaceutics 221 (2001) Review Biomedical applications of collagen Chi H. Lee a, *, Anuj Singla a, Yugyung Lee b a Department of Pharmaceutics, College of Pharmacy, The Uni ersity of Missouri-Kansas City, 5005 Rockhill Rd, Katz Bdg c108, Kansas City, MO 64110, USA b School of Interdisciplinary Computing and Engineering, The Uni ersity of Missouri-Kansas City, Kansas City, MO 64110, USA Received 5 January 2001; received in revised form 26 March 2001; accepted 3 April 2001 Abstract Collagen is regarded as one of the most useful biomaterials. The excellent biocompatibility and safety due to its biological characteristics, such as biodegradability and weak antigenecity, made collagen the primary resource in medical applications. The main applications of collagen as drug delivery systems are collagen shields in ophthalmology, sponges for burns/wounds, mini-pellets and tablets for protein delivery, gel formulation in combination with liposomes for sustained drug delivery, as controlling material for transdermal delivery, and nanoparticles for gene delivery and basic matrices for cell culture systems. It was also used for tissue engineering including skin replacement, bone substitutes, and artificial blood vessels and valves. This article reviews biomedical applications of collagen including the collagen film, which we have developed as a matrix system for evaluation of tissue calcification and for the embedding of a single cell suspension for tumorigenic study. The advantages and disadvantages of each system are also discussed Elsevier Science B.V. All rights reserved. Keywords: Collagen; Biomaterial; Drug/protein/gene delivery; Tissue engineering 1. Introduction * Corresponding author. Tel.: ; fax: address: (C.H. Lee). Collagen, a well-known protein, has been widely used in medical applications. Many natural polymers and their synthetic analogues are used as biomaterials, but the characteristics of collagen as a biomaterial are distinct from those of synthetic polymers mainly in its mode of interaction in the body (McPherson et al., 1986). Collagen plays an important role in the formation of tissues and organs, and is involved in various functional expressions of cells. Collagen is a good surface-active agent and demonstrates its ability to penetrate a lipid-free interface (Fonseca et al., 1996). Collagen exhibits biodegradability, weak antigenecity (Maeda et al., 1999) and superior biocompatibility compared with other natural polymers, such as albumin and gelatin /01/$ - see front matter 2001 Elsevier Science B.V. All rights reserved. PII: S (01)
2 2 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) 1 22 The primary reason for the usefulness of collagen in biomedical application is that collagen can form fibers with extra strength and stability through its self-aggregation and cross-linking. In most of drug delivery systems made of collagen, in vivo absorption of collagen is controlled by the use of crosslinking agents, such as glutaraldehyde (Barbani et al., 1995), chromium tanning (Bradley and Wilkes, 1977), formaldehyde (Ruderman et al., 1973), polyepoxy compounds (Tu et al., 1993), acyl azide (Petite et al., 1990), carbodiimides (Nimni et al., 1988), and hexamethylenediisocyanate (Chvapil et al., 1993). Physical treatment, such as ultra-violet/ gamma-ray irradiation and dehydrothermal treatment, have been efficiently used for the introduction of crosslinks to collagen matrix (Harkness 1966; Stenzel et al., 1969; Miyata et al., 1971; Gorham et al., 1992). The thiolation of denatured collagen, which allows precise amounts of SH groups to be attached onto the protein backbone, was also investigated (Nicholas and Gagnieu, 1997). It was reported that, under optimized conditions, oxidized and denatured thiolated collagen films are more resistant and rigid than glutaraldehyde treated ones. The use of collagen as a drug delivery system is very comprehensive and diverse. Collagen can be extracted into an aqueous solution and molded into various forms of delivery systems. The main applications of collagen as drug delivery systems are collagen shields in ophthalmology (Kaufman et al., 1994), sponges for burns/wounds (Rao, 1995), mini-pellets and tablets for protein delivery (Lucas et al., 1989), gel formulation in combination with liposomes for sustained drug delivery (Fonseca et al., 1996), as controlling material for transdermal delivery (Thacharodi and Rao, 1996), and nanoparticles for gene delivery (Rossler et al., 1995). In addition, its uses as surgical suture (Miller et al., 1964), hemostatic agents (Cameron, 1978; Browder and Litwin, 1986), and tissue engineering including basic matrices for cell culture systems (Kemp, 2000) and replacement/substitutes for artificial blood vessels and valves (Chvapil et al., 1993; Auger et al., 1998; Huynh et al., 1999) were reported earlier. Due to its excellent biocompatibility and safety, the use of collagen in biomedical application has been rapidly growing and widely expanding to bioengineering areas. However, some disadvantages of collagen-based systems arose from the difficulty of assuring adequate supplies, their poor mechanical strength, and ineffectiveness in the management of infected sites (Friess, 1998). Improvement of the physical, chemical and biological properties will be necessary to address some of drawbacks in collagen based applications. The better collagen delivery systems having an accurate release control can be achieved by adjusting the structure of the collagen matrix or adding other proteins, such as elastin, fibronectin or glycosaminoglycans (Doillon and Silver, 1986; Lefebvre et al., 1992, 1996). A combination of collagen with other polymers, such as collagen/liposome (Kaufman et al., 1994; Fonseca et al., 1996) and collagen/silicone (Suzuki et al., 2000), has been proposed to achieve the stability of a system and the controlled release profiles of incorporated compounds. The purpose of this article is to review biomedical applications of collagen including the collagen film, which we have developed as a matrix system for evaluation of tissue calcification and controlled delivery of cardiovascular drugs. This collagen matrix system further serves as the substrate for the embedding of a single cell suspension or a small tumor specimen in the evaluation process of cancer therapy. The advantages and disadvantages of each system are also discussed. 2. Characterization of collagen as a biomaterial Collagen is the primary structural material of vertebrates and is the most abundant mammalian protein accounting for about 20 30% of total body proteins (Harkness, 1961). It is present in tissues of primarily mechanical function. About one half of the total body collagen is in the skin and about 70% of the material other than water present in dermis of skin and tendon is collagen. Collagen made its appearance at the early stage of evolution in such primitive animals as jellyfish, coral and sea anemones (Bergeon, 1967). Collagen is synthesized by fibroblasts, which usually originate from pluripotential adventitial cells or reticulum cells.
3 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) The molecular structure of collagen has been firmly established on the evidence from earlier studies, such as amino acid composition analysis, X-ray diffraction analysis, electron microscopy and physicochemical examination of solutions (Gross, 1963; Ramachandran and Sasisekharan, 1965; Burge, 1964). Collagen has a unique structure, size and amino acid sequence (Miyata et al., 1992; Rao 1995). The collagen molecule consists of three polypeptide chains twined around one another as in a three-stranded rope. Each chain has an individual twist in the opposite directions. The principal feature that affects a helix formation is a high content of glycine and amino acid residues (Piez, 1984). The strands are held together primarily by hydrogen bonds between adjacent CO and NH groups, but also by covalent bonds (Harkness, 1966). The basic collagen molecule is rod-shaped with a length and a width of about 3000 and 15 A, respectively, and has an approximate molecular weight of 300 kda (Traub and Piez, 1971; Nimni and Harkness, 1988). At least 19 types of collagen have been reported. Types I, II and III collagen as well as types V and XI are built up of three chains and all are composed of the continuous triple-helical structure. Types I, II, III, and V are called as fibril forming collagens and have large sections of homologous sequences independent of species (Timpl, 1984). In type IV collagen (basement membrane), the regions with the triplehelical conformation are interrupted with large non-helical domains as well as with the short non-helical peptide interruption. Fibril associated collagens (Type IX, XI, XII and XIV) have small chains, which contain some non-helical domains. Type VI is microfibrilla collagen and type VII is anchoring fibril collagens (Samuel et al., 1998). An investigation on the native collagen has led to a better understanding of a structure function relationship between target drugs and collagen. A three-dimensional (3-D) model of fibril-forming human type II collagen was proposed for the development of synthetic collagen tissues and the study of the structural and functional aspects of collagen (Chen et al., 1995). This system also allows the studies of the stereochemistry of all the side chain groups and specific atomic interactions, and further evaluation of its therapeutic effects on collagen related diseases. The orderly arrangement of triple helix tropocollagen molecules results in a formation of fibrils having a distinct periodicity. Nonhelical telopeptides are attached to both ends of the molecule and serve as the major source of antigenecity. Atelocollagen, which is produced by elimination of the telopeptide moieties using pepsin, has demonstrated its potential as a drug carrier, especially for gene delivery (Kohmura et al., 1999; Ochiya et al., 1999). Table 1 summarizes the major characteristics of collagen, which are suitable for medical applications (Jerome and Ramshaw, 1992; Rao, 1995; Friess, 1998; Fujioka et al., 1998; Maeda et al., Table 1 Advantages and disadvantages of collagen as a biomaterial a Ad antages Available in abundance and easily purified from living organisms (constitutes more than 30% of vertebrate tissues); Non-antigenic; Biodegradable and bioreabsorbable; Non-toxic and biocompatible; Synergic with bioactive components; Biological plastic due to high tensile strength and minimal expressibility; Hemostatic promotes blood coagulation; Formulated in a number of different forms; Biodegradability can be regulated by cross-linking; Easily modifiable to produce materials as desired by utilizing its functional groups; Compatible with synthetic polymers; Disad antages High cost of pure type I collagen; Variability of isolated collagen (e.g. crosslink density, fiber size, trace impurities, etc.); Hydrophilicity which leads to swelling and more rapid release; Variability in enzymatic degradation rate as compared with hydrolytic degradation; Complex handling properties; Side effects, such as bovine spongeform encephalopathy (BSF) and mineralization a Sources; Jerome and Ramshaw, 1992; Rao, 1995; Friess, 1998; Fujioka et al., 1998.
4 4 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) ). It is easily absorbable in the body and has very low antigenicity. It has high tensile strength and high affinity with water. Moreover, it is nontoxic, biocompatible and biodegradable (Friess, 1998; Maeda et al., 1999). It can be prepared in a number of different forms including strips, sheets, sponges and beads. Collagen can be solubilized into an aqueous solution, particularly in acidic aqueous media, and can be engineered to exhibit tailor-made properties. Collagen is relatively stable due to its function as the primary structural protein in the body, but it is still liable to collagenolytic degradation by enzymes, such as collagenase and telopeptide-cleaving enzymes (Woolley, 1984). Collagenase binds tightly to triple helices, and degrades collagen starting from the surface. The melting profile of the pepsin-solubilized collagen showed a biphasic transition, indicating that age-related decrease in thermal stability has implications for the mechanical strength and turnover of the bone collagen (Danielsen, 1990). Reports of adverse reactions to collagen have been restricted to localized redness and swelling following plastic surgery using collagen implants and wound breakdown with the use of catgut suture material (Webster et al., 1984; Carrol, 1989). Clinical reactions to collagen were rare, but two cases of allergic (IgE-mediated) reactions to bovine collagen were reported (Mullins et al., 1996). Patients in both cases developed conjunctive edema in response to the topical application of highly purified bovine collagen to eye during ophthalmic surgery. When irritant effects and cytotoxicity of various products developed from collagen were evaluated, cell response to exogenous collagen starts shortly after the material is kept in contact with tissues, evoking a local and fast inflammatory response, whose intensity depends on the pharmaceutical formulation in use (Trasciatti et al., 1998). Even though, unknown reverse effects may be discovered in the future application of collagen for gene delivery or tissue engineering, since collagen can help to avoid side effects originated from incorporated drugs, therapeutic peptides and proteins, the need for the continuous effort in development and evaluation of collagen based systems is manifest. 3. Collagen-based drug delivery systems 3.1. Film/sheet/disc The main application of collagen films is as barrier membrane. Films with the thickness of mm and made of biodegradable materials, such as prepared from telopeptide-free reconstituted collagen, demonstrated a slow release profile of incorporated drugs (Rubin et al., 1973). The drugs can be loaded into collagen membranes by hydrogen bonding, covalent bonding or simple entrapment. They can be sterilized and become pliable upon hydrolyzation, while retaining adequate strength to resist manipulation. When collagen film was applied to eye, it was completely hydrolyzed after 5 6 h (Bloomfield et al., 1978). This finding adds to evidence that collagen-based systems are suitable for resembling current liquid and ointment vehicles. Collagen film/sheet/disc have been used for the treatment of tissue infection, such as infected corneal tissue or liver cancer. Soluble ophthalmic insert in the form of a wafer or a film was introduced as a drug delivery system for the treatment of infected corneal tissue using a high dose of antibiotic agents, such as gentamicin (Bloomfield et al., 1978) and tetracycline (Minabe et al., 1989a). The wafer route of administration gave the highest tissue concentration of incorporated drugs. The duration of therapeutic effect after administration of the collagen film containing tetracycline demonstrated that tetracycline could be detected in the plasma for more than 7 days after implantation into rabbits (Minabe et al., 1989a,b). The microfibrous collagen sheets as a local delivery carrier for the treatment of cancer was evaluated (Sato et al., 1996). The local application of collagen sheets loaded with anticancer agent, ectopocide (VP-16), resulted in a relatively long maintenance of drug concentrations at the target site, which, in this case, is the liver. Some modifications on collagen film/sheet/disc have been made to control the release rate of incorporated drugs from delivery systems. Collagen films crosslinked by chromium tanning, formaldehyde or a combination of both have been successfully used as implantable delivery systems
5 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) in achieving the sustained release of medroxyprogesterone acetate (Bradley and Wilkes, 1977). A modification by attaching another membrane to collagen based film/sheet/disc was attempted to achieve the controlled release rate of incorporated drugs. A transdermal delivery device containing nifedipine, whose release rate was well controlled by an attached membrane made of chitosan, showed the highest therapeutic efficacy in the treatment of tissue infection (Thacharodi and Rao, 1996). Collagen film and matrix were used as gene delivery carriers for promoting bone formation. A composite of recombinant human bone morphogenetic protein 2 (rhbmp-2) and collagen was developed to monitor bone development and absorbent change of carrier collagen (Murata et al., 1999, 2000). The rhbmp-2/collagen onlay implant resulted in active bone formation, whereas the collagen alone resulted in no bone formation. Collagen provides an anchorage for cell differentiation and remains as an artificial matrix in woven bone. In a similar study, collagen matrix loaded with BMP and placed in a close contact with osteogenic cells achieved direct osteoinduction without causing a cartilage formation (Nakagawa and Tagawa, 2000). These results indicate that a collagen based gene delivery system is very efficient as a biological onlay implant. Collagen film and disc as gene delivery systems have many advantages. Systems that isolate transplanted cells from the host immune system might be beneficial and economically attractive, because they would allow the use of allogenic or even xenogenic cells in many patients (Liu et al., 1993; Al-Hendy et al., 1996; Tani et al., 1989; Brauker et al., 1995). The use of genetically modified cells for a long-term delivery of a therapeutic transgene product has been an attractive option for the treatment of monogenetic hereditary as well as many multifactorial nongenetic diseases (Barr and Leiden, 1991; Scharfmann, et al., 1991; Heartlein, et al., 1994). Biodegradable collagen films or matrices have served as scaffolds for a survival of transfected fibroblasts (Rosenthal and Kohler, 1997). While these methods seem to allow an adequate cell survival, the concerns about long-term biocompatibility of non-degradable materials also arose. In several animal models, a long-term expression of a foreign gene after implantation of transfected cells has not been achieved (Aebischer et al., 1996). A combination of collagen and other polymers, such as atelocollagen matrix added on the surface of polyurethane films, enhanced attachment and proliferation of fibroblasts and supported growth of cells (Park et al., 2000). Transplantation of cells embedded in a lattice of polytetrafluoroethylene fibers coated with rat collagen followed by a mixing with matrigel as well as basic fibroblast growth factor showed that a long-term expression of human -glucuronidase by retroviral-transduced murine or canine fibroblasts was achievable using a collagen-based matrix system. (Moullier et al., 1993a,b, 1995). Therefore, collagen-based film/disc systems seem to need to contain extra matrices that improve conditions for a long-term cell survival Collagen film as a calcifiable matrix system One of the problems with implantable biomaterials is their calcification, which is influenced by structure of the implantable system, and determines its in vivo therapeutic efficiency and clinical fate (Schoen et al., 1992). Calcification of tissue or systems depends on chemical factors that operate at the cellular level around various tissues or biomaterials (Wada et al., 1999). Both collagen and elastin are major components of connective tissues, which possess a structure that compromises collagen fibers intimately associated with a remarkably stable elastin network. The suitability of collagen and elastin in many potential medical applications in reconstructive and plastic surgery including controlled delivery of bone morphogenetic protein has been reported (Vardaxis et al., 1996). In our laboratory, the matrix films, which are composed of various combinations of collagen and elastin, have been developed and evaluated for its uses in tissue calcification and as a controlled delivery device for cardiovascular drugs. Collagen films, which we have developed, were used to simulate the calcification process of implantable biomaterials, such as bioprosthetic heart
6 6 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) 1 22 valve (BHV). In BHV, the aortic wall and leaflet have mainly served as calcifiable matrix. Recently, the calcification of the bioprosthetic aortic wall has been extensively studied due to increasing use of the stentless BHV. The stentless BHV has a relatively large segment of exposed aortic wall comparing to the stented valve, in which virtually no aortic wall is exposed outside the stent. Thus, bioprosthetic aortic wall calcification has a potential to cause the clinical failure of the stentless BHV. Aortic wall is composed of 90% collagen and 10% of elastin, while leaflet is mainly composed of collagen (99%). Due to their differences in composition, the calcification rates of aortic wall and leaflet and their response to anti-calcification agents are different. For example, ethanol pretreatment completely inhibited calcification of porcine leaflet, while only partially (about 50%) inhibited calcification of porcine aortic wall (Lee et al., 1998). This may indicate that elastin has a more critical role in tissue calcification than collagen. This result has led to investigation of the elastin concentration effects on the calcification rate of implantable biomaterials. Collagen films made of various combinations of collagen and elastin were evaluated for their suitability as drug delivery systems. Biomaterials should possess mechanical properties capable of withstanding the forces and motions experienced by the normal tissues and have sufficient fatigue strength to ensure a long life of the implant in vivo (Meaney, 1995). Tensile strength can be used for evaluation of mechanical strength, resilient activity, endurance and biocompatibility of the systems. Collagen films, we have developed, has a size of 6 10 mm and a thickness of 1 mm. Its tensile strength was determined using the following equation, Force or load (F) Tensile strength ( )= MA where F is the maximum load (in Newton) and MA is the minimum cross-sectional area of the film specimen (in square meters) (Fell and Newton, 1970). Chatillon DFM-10 Gauge equipped with LTC Manual Test Stand and GF-1 Grips (Ametek Test & Calibration Instruments Division, Largo, FL) was used. The tensile strength Table 2 The tensile strength of films containing various combinations of collagen and elastin a FILM Composition (Collagen:Elastin) Tensile Strength (MPa S.D.) 90: : : a N=6 each. Values are not significantly different. was almost constant irrespective of a loading ratio of collagen and elastin and within a durable range as shown in Table 2. There was no sign of swelling of the system, which is a sensitive marker of collagen deterioration (Bank et al., 2000). This system was well endurable after subcutaneous implantation in the rat for up to three weeks and no side effect or infection was detected. As shown in Fig. 1, as the concentration of elastin in a system increased from 10 to 90%, the total amount of calcium accumulation in a system implanted in the rat subcutaneous model also increased. This result indicates that elastin has a more critical role in tissue calcification than collagen and that this system can be used as a calcifiable matrix simulating calcification process of implantable tissues, such as BHV. This system can be further applicable to local and systemic delivery of various anticalcification agents, cardiovascular drugs and antibiotics for the treatment of heart diseases. The collagen-based matrix, we have developed, can be used as a lattice for tissue culture systems. In the collagen based culture system, a film prepared from collagen fiber provides the substrate for the embedding of a single cell suspension or a small tumor specimen. Three-dimensional aggregates can be kept viable and proliferating for weeks, demonstrating very good degrees of resemblance compared with the in vivo tumors from which they were derived. The matrix remained stable in shape and size during the cell culture. The three-dimensional models show more resistance to treatment with anticancer drugs than cells growing as monolayers. They can serve as better models for the biological and biochemical characteristics of human solid tumors than monolayer subconfluent cell cultures. Collagen-based
7 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) matrix cultures offer unique opportunities for the study of the mechanisms behind human tumor progress Collagen shields The collagen shield was originally designed for bandage contact lenses, which are gradually dissolved in cornea (Wedge and Rootman, 1992). The idea of using a shield or a hydrogel lens as a delivery device has led to the development of various drug delivery systems for ophthalmic applications. One of the merits of the collagen-based drug delivery systems is the ease with which the formulation can be applied to the ocular surface and its potential for self administration (Friedberg et al., 1991; Lee, 1990). The collagen corneal shield is fabricated from porcine sclera tissue that closely resembles collagen molecules of the human eye (Harrison, 1989). The mechanical properties of the shield protect the healing corneal epithelium from the blinking action of the eyelids (Mondino, 1991). The collagen corneal shield would promote epithelial healing after corneal transplantation and radial keratomy (Robin et al., 1990; Shaker et al., 1989; Marmer 1988; Poland and Kaufman, 1988; Waltman and Kaufman, 1970; Unterman et al., 1988). Drug delivery by collagen shields depends on loading and a subsequent release of medication by the shield (Leaders et al., 1973). The collagen matrix acts as a reservoir and the drugs are entrapped in the interstices of the collagen matrix in a solution for water-soluble drugs or incorporated into the shield for water-insoluble drugs. As tears flush through the shield and the shield dissolves, it provides a layer of biologically compatible collagen solution that seems to lubricate the surface of the eye, minimize rubbing of the lids on the cornea, increase the contact time between the drug and the cornea, and foster epithelial healing (Kaufman, 1988; Kaufman et al., 1994). A bolus release of drug from the lenses was attributable to the enhanced drug effect (Waltman and Kaufman, 1970; Podos et al., 1972). Therefore, this system allows the higher corneal concentrations of drug, and the more sustained drug delivery into the cornea and the aqueous humor. As shown in the Table 3, collagen shields were used as delivery devices for the treatment of various local infections and their therapeutic effects were compared with the conventional formula- Fig. 1. The Effect of ethanol or gramicidin on the calcification rates of porcine aortic wall implanted in rat subcutaneous models (N=6).
8 8 C.H. Lee et al. / International Journal of Pharmaceutics 221 (2001) 1 22 Table 3 The application of collagen shields for various topical agents Drugs/Agents Reference Antibiotics Gentamicin Bloomfield et al., 1978; Baziuk et al., 1992; Liang et al., 1992; Milan et al., 1993 Vancomycin Phinney et al., 1988 Tobramycin O Brien et al., 1988; Poland and Kaufman, 1988; Unterman et al., 1988; Aquavella et al. 1988; Hobden et al., 1988; Sawusch et al., 1988a,b; Assil et al., 1992 Netilimycin Dorigo et al., 1995 Polymyxin B Sulfate Palmer and McDonald, 1995 Trimethoprim Palmer and McDonald, 1995 AmphotericinB Schwartz et al., 1990; Mendicute et al., 1995 Trifluorothymidine Gussler et al., 1990 Acyclovir Willey et al., 1991 Ofloxacin Taravella et al., 1999 Steroids Aquavella et al., 1988; Sawusch et al., 1988a,b; Hwang et al., 1989; Milan et al., 1993; Palmer and McDonald, 1995 Cholinergic: Pilocarpine Aquavella et al., 1988 Antineoplastic: 5-fluorouracil Finkelstein et al., 1991 Anticoagulant: Heparin Murray et al., 1990 Immunodepressant Cyclosporin Chen et al., 1990; Reidy et al., 1990; Sato et al., 1996; Gebhardt and Kaufman, 1995 Gene therapy Plasmid DNA Angella et al., 2000 tions. The use of antibiotic collagen shields supplemented by frequent topical applications has been clinically useful for preoperative and postoperative antibiotic prophylaxis, the initial treatment of bacterial keratitis, and the treatment of corneal abrasions (Poland and Kaufman, 1988; Friedberg et al., 1991). Most of these studies showed that shields provided equal or better drug delivery of fluorescein (Reidy et al., 1990), prednisolone acetate (Sawusch et al., 1988a,b), cyclosporine (Reidy et al., 1990), and ofloxacin (Taravella et al., 1999) to the anterior segment. Delivery of drugs through the impregnated collagen shield was more comfortable and reliable than frequent application of other conventional treatments, such as drops, ointment or daily subconjunctive injection (Friedberg et al., 1991). An application of collagen shield was extended to gene delivery area. Delivery of plasmid DNA into the bleb through a collagen shield increased chloramphenicol acetyltransferase, the reporter gene, 30-fold over injection of plasmid DNA through saline vehicle (Angella et al., 2000). Gene therapy using naked plasmid DNA and a simple collagen shield delivery was very useful for regulating wound healing after glaucoma surgery. Modifications of collagen were made to simplify the application, to meet the highest compliance, to reduce blurring of vision, and to enhance the drug concentration and bioavailability of drugs in the cornea and aqueous humor (Kuwano et al., 1997). The cross-linked collagen using glutaraldehyde or chromium tanning can serve as a drug reservoir and provide more desirable drug delivery than non cross-linked collagen shields by increasing the contact time between the drug and the cornea. Collasomes, in the form of collagen pieces, were developed by adding long hydrocarbon side chains to the collagen (Kaufman et al., 1994). This modification increases not only the hydrophobicity of the collagen but also the total surface area, which effectively decreases the diffusion rate of hydrophilic drug molecules from the collagen matrix. Collasomes can be formulated with various constituents and chemically alternated with the addition of lipid (called Lacrisomes) for the treatment of dry eyes (Kaufman et al., 1994). In this work, a delivery system in which collagen pieces were suspended in a viscous vehicle was instilled into the lower forniceal space. Collasomes hydrated in a solution of sodium fluorescein and suspended in a methylcellulose vehicle as a model for delivery of water-soluble drugs produced fluorescein concentrations much higher in the cornea and aqueous humor, comparing with fluorescein-containing vehicle alone.